# Metamaterials and imaging

- Minkyung Kim
^{1}and - Junsuk Rho
^{1, 2}Email author

**Received: **20 April 2015

**Accepted: **22 June 2015

**Published: **9 November 2015

## Abstract

Resolution of the conventional lens is limited to half the wavelength of the light source by diffraction. In the conventional optical system, evanescent waves, which carry sub-diffraction spatial information, has exponentially decaying amplitude and therefore cannot reach to the image plane. New optical materials called metamaterials have provided new ways to overcome diffraction limit in imaging by controlling the evanescent waves. Such extraordinary electromagnetic properties can be achieved and controlled through arranging nanoscale building blocks appropriately. Here, we review metamaterial-based lenses which offer the new types of imaging components and functions. Perfect lens, superlenses, hyperlenses, metalenses, flat lenses based on metasurfaces, and non-optical lenses including acoustic hyperlens are described. Not all of them offer sub-diffraction imaging, but they provide new imaging mechanisms by controlling and manipulating the path of light. The underlying physics, design principles, recent advances, major limitations and challenges for the practical applications are discussed in this review.

## Keywords

## 1 Introduction

Curiosity and desire to see microscopic world have leaded the invention of the optical microscope. Thanks to the optical microscope, the small structures that had been invisible to the naked eyes could be seen. Modern biology and medical science where large portions are based on the observation of micro-objects such as cells and bacteria have been developed with the advance in the optical microscope. With fluorescent materials, optical microscopes became more useful and essential for the decades, but there is still a fundamental question how to achieve the spatial resolution below diffraction limit.

In 1870s, Abbe discovered that when an object is observed by optical devices such as microscopes or telescopes, the features smaller than half of the wavelength of light are not resolvable because of diffraction phenomena [1]. Due to diffraction limit, resolution achievable by using conventional optical microscope is intrinsically limited to approximately two hundred nanometers in visible light. Realizing microscopes with higher resolution have been active research area. At 1930s, microscopes using electrons such as scanning electron microscope (SEM) [2] and transmission electron microscope (TEM) [3] were invented. Those two microscopes have much higher resolutions of tens of nanometers compared to the typical optical microscope due to the shorter de Broglie wavelength of electrons. However, since studying living specimens is not compatible with the electrons in general, the electron microscopes are inadequate for the biological applications although they are the most common imaging tools to visualize the nanoscale structures. Around the same time, near-field scanning optical microscope (NSOM) in which evanescent waves are obtained by putting detector very close to an object was proposed [4, 5]. Lateral resolution of 20 nm and vertical resolution of 2–5 nm have been achieved [6, 7]. However, long scanning time and tricky conditions such as very short distance between the detector and the object were the obstacles for the practical imaging applications. At 1980s, the spatial resolution of order of few nanometers was realized by atomic force microscopy (AFM) [8, 9]. AFM has many advantages including capability of 3D imaging and compatibility in liquid environment, but very small single scanning size and ow scanning speed raised problems. The biggest limitation of NSOM and AFM is that both do topography imaging which examines only the surface in the near-field.

To overcome such limitations, far-field microscopy with super-resolution and bio-compatibility have been successfully developed and widely used. Localization microscopy techniques such as stochastic optical reconstruction microscopy (STORM) [10] and photo activated localization microscopy (PALM) [11, 12] using photoswitchable fluorophores were proposed. And, as non-localization approaches, stimulated emission depletion (STED) [13] microscopy using two laser pulses to achieve 3D/multi-color/video-rate imaging accomplished 6 nm spatial resolution [14]. Saturated structured-illumination microscopy (SSIM) [15] using nonlinear dependence of fluorophores and structured illumination microscopy (SIM) [16] using grid patterned incident light have been also developed. However, for the microscopes using laser, samples can be damaged by high-intensity pulse of the laser, and for the microscopes based on fluorescent materials, resolutions are limited by the labeling density and the size of the fluorescent labels [17]. In addition to the development of such advanced imaging methods, various algorithms and techniques to realize super-resolution have been also studied [18].

In this review, we will describe the new types of imaging approaches based on new optical materials called metamaterials which can provide the direct control and manipulation of electromagnetic properties to overcome diffraction limit. Metamaterial-based imaging composed with the special lenses, for example, but not limited to, superlenses, hyperlenses, metalenses, and non-optical lenses such as acoustic hyperlens will be reviewed, and the underlying physics, design principles, recent advances, major limitations and challenges for the practical applications will be discussed in each section. Since the lenses are named by proposers, not by social protocols, the boundaries of the divided groups may be ambiguous.

## 2 Review

### 2.1 To overcome diffraction limit

*k*

_{⊥}) are bounded. Evanescent waves have higher

*k*

_{⊥}than the bounded value, and therefore, they carry sub-diffraction information. However, since the propagating component (

*k*

_{∥}) is imaginary from the dispersion relation, the amplitude will exponentially decay and the sub-diffraction information cannot reach to the image plane.

Meanwhile, materials with hyperboloid isofrequency surface, as shown in Fig. 1 (b) and (c), can deal with the evanescent waves since *k*
_{⊥} can have unbounded value. More generally, if there exists a lens in which the evanescent waves can be transferred from the object plane to the image plane without exponential decay, diffraction limit could be overcome. In addition, if impedance of the lens is matched to one of air so that all the incident light are transmitted through the lens without any reflection, every beam from the object plane will reach the image plane. It indicates that theoretically perfect lens with infinite resolution can be realized. Such a perfect lens has been proposed and studied by metamaterials.

Metamaterials are artificially structured materials composed of the building blocks of which size and spacing of atoms are at deep sub-wavelength scale. Their extraordinary electromagnetic responses are determined by the size, shape and arrangement of the unit cells, not by chemistry. By arranging those building blocks properly, metamaterials exhibit fascinating optical properties that do not exist in nature such as negative refractive index, invisibility cloak, artificial chirality, superlensing and hyperbolic dispersion relation.

Negative index materials (NIMs), one of the most interesting applications of metamaterials, were first proposed by Veselago in 1960s. He predicted that a hypothetic material where both ε and μ are negative has negative refractive index. At the interface of positive index medium and negative index medium, light will be negatively refracted and the energy and phase will flow in the opposite direction in the medium of negative index. It was also noted that negative refraction causes many other unusual phenomena such as reversed Doppler/Cherenkov effect [19].

Thanks to such extraordinary optical properties, metamaterials have shown great potentials in many applications including waveguide [34, 35], artificial magnetism [37], spontaneous emission enhancement [38], and transformation optics [39, 40], and one of the most exciting applications is the diffraction-free imaging which is also called sub-diffraction or super-resolution imaging.

### 2.2 Perfect lens from negative index

The first theoretical study about sub-diffraction imaging using metamaterials was done by Pendry [41, 42]. He proposed that a NIM slab with ε = μ = − 1 works as a perfect lens. There had been many debates on whether it is a true perfect lens or not because the slab does not look like a lens; it only works for an object placed on a certain distance and has no focal length [43]. But, NIM slab as a perfect lens was theoretically and experimentally demonstrated in many research groups [24, 25, 41, 44, 45].

*k*

_{∥}changes at the interface of a positive index and negative index medium as indicated in Fig. 3 from the causality principle and conservation of transverse wavevectors. Evanescent wave which was exponentially decaying is now exponentially increasing in NIMs. In short, evanescent wave is amplified and travels further in NIMs comparing in the positive-index materials, as shown in Fig. 4 (b) [41, 46].

From the reversal of phase and energy flow, phase of propagating wave goes backwards as the ray goes forward, cancelling out phase gained through the same thickness of vacuum. Phase of propagating wave and amplitude of the evanescent wave are restored. Furthermore, all incident light transmits the NIM slab without reflection since the NIM slab and air have identical impedance value. Therefore, a NIM slab that has n = −1 can be considered as a perfect lens in which the image and the object are exactly the same.

Microscopically explaining, amplification of evanescent wave stems from surface resonance [41, 47–50]. When TM waves enter an interface across which the sign of the permittivity is different, oscillation of electron density, called surface plasma oscillation, is generated. If surface mode and the wavevectors of evanescent waves are matched, surface plasmon resonance occurs, generating electromagnetic waves with shorter wavelength that propagate along the interface. These waves, or surface plasmon polaritons (SPPs), have amplitude exponentially decaying along the transverse axis. Since the waves have shorter wavelength than the incident light, light can be tightly confined in a subwavelength size area and the local field intensity can be enhanced significantly. In the process, the evanescent waves are enhanced, leading to sub-diffraction limit imaging.

### 2.3 Near-field superlens from negative permittivity

The ideal condition to be a perfect lens was ε = μ = − 1, if the dielectric background is air. However, when dealing with very near field or when all dimensions are much smaller than the wavelength of interest, quasistatic limit can be applied. Electric field and magnetic field are decoupled, and the electric and magnetic responses can be considered to be independent. Then under one certain polarization condition, either one of permittivity and permeability negative is sufficient to realize perfect imaging. For TM wave, only negative permittivity (ε < 0, μ > 0) is enough as well [41]. (Note that it is equal to existence condition of SPPs).

*ω*

_{ p }due to the collective response of free electrons.

*ω*

_{ p }, a plasma frequency, is normally around ultraviolet (UV) regime for metals. Such a negative permittivity material slab with the thickness much smaller than the wavelength functions as a super-resolution lens, and therefore, is called “superlens” [51]. The first experimental sub-diffraction imaging using superlens was demonstrated in near-field images with 60 nm half-pitch resolution in UV range as shown in Fig. 5 [52].

Though evanescent waves are enhanced, metals’ high resistive losses from the imaginary part of permittivity degrade the image, which is the main limiting factor of the infinite resolution. Thanks to its relatively low losses, silver has been studied as a material for a superlens [41]. Amplification of evanescent waves was numerically [49, 53] and experimentally [48, 49, 53, 54] demonstrated in a thin silver film. Resolution of one-sixth of the incident wavelength at the UV frequency region using silver [52, 55], and resolution of a twentieth of the incident wavelength at mid-IR frequency range using SiC [56] were achieved through numerical simulation and experimental demonstration, respectively. Other designs of superlenses including a silver slab bounded by two different positive index media [47] have been also proposed.

There have been lots of studies to reduce losses in plasmonics materials [57–59]. Use of gain media, materials with negative imaginary part of refractive index, to compensate the losses [60], diluted metals [61, 62], highly doped semiconductors [63, 64], and even superlenses without metal [65] to reduce ohmic-related losses have been proposed since high carrier concentration induces high losses. Nevertheless, high losses were still huge limitations for the practical imaging applications of the superlenses. To minimize losses, the researches to find optimal film thickness and surface roughness requirements that transmit maximum intensity were conducted [42, 49, 52, 66] and moreover, placing multiple thin superlenses to reduce the propagation length in the superlens was proposed [67, 68].

Another limitation of superlenses is polarization dependence. As mentioned earlier, surface plasmons, that are responsible for sub-diffraction imaging, are excited in TM condition. Thus, the superlenses work only for TM wave. Resonance based characteristics also give rise to narrow frequency bandwidth. Working frequency of superlenses has been extended to the mid-IR region [69–71], and multi-wavelength superlens consisting of multilayer of polar dielectric materials exhibiting sub-diffraction imaging in three simultaneous frequencies was also presented [72], while the bandwidths of the individual superlenses are still narrow. Projection type of image with the same size to the object, i.e. no magnification is also one of the limitations. But, the biggest disadvantage is that superlenses work only in the near-field [41, 68]. The distance between the lens and the image plane has to be very short as well as the distance between a source and the lens since evanescent waves decay exponentially again after they passes through the superlens. It prevents the practical super-resolution imaging applications of superlenses.

### 2.4 Far-field superlens

For the far-field sub-diffraction imaging, evanescent waves have to be not only amplified, but also converted into propagating waves. It is fairly similar to the near-field superlens except that there are subwavelength scale periodic metallic gratings on the exit surface. It was proven that under TM condition, a periodic metallic corrugation on the lens surface couples evanescent waves and propagating waves [73].

As the evanescent waves from the object transmit through a nanopatterned superlens, the near-field image and the grating pattern are overlapped, generating a moiré pattern, an interference pattern created when two periodic or quasi-periodic patterns are superimposed [77, 78]. The spatial frequency of the moiré pattern is equal to the difference of the frequency of the evanescent wave and the grating pattern. Even if either the evanescent waves or the grating is not resolvable due to diffraction limit, the moiré pattern can be resolved if it has lower wavevector than the spatial resolution. Therefore, the near-field image can be numerically reconstructed by analyzing moiré fringes as long as the grating pattern is known [79]. Since period of the grating pattern is limited only by fabrication, not by diffraction, super-resolution which had been impossible before was realized [76].

More generally, the near-field and far-field angular spectrum has a one-to-one relationship, following the grating law. Transverse wavevectors of transmitted propagating waves (*k*
^{'}) can be expressed in terms of transverse wavevectosr of the incident evanescent wave (*k*) and the grating wave number (*G*): *k*
^{'} = *k* + *pG*, where *p* is the diffraction order [73]. When *p* is negative and the grating wavenumber is large enough, the wavevectors of the transmitted waves is reduced enough to propagate, resulting in far-field sub-diffraction imaging. Transmission of sub-diffraction image through near-field superlens and far-field superlens when the diffraction order is equal to −1 are illustrated in Fig. 6 (a) and (b), respectively [73].

The image, obtained as a field angular spectrum, has to be transformed into a real space image via inverse Fourier transformation. It makes real time imaging impossible, which is the main obstacle of FSL imaging [73]. To achieve real time imaging, a FSL with a different mechanism which functions for a certain range of wavevectors was investigated [74, 75]. Also, the earlier researches have focused on UV region, but the wavelength range was expanded to visible frequencies by changing permittivity of the materials [80].

By investigating absorption and transmission factor for TM and TE waves, another research revealed that the conversion of evanescent waves into propagating waves in FSL results from excitation of SPPs supported by the metallic grating. Incident TM waves scattered at the exit surface excite SPP modes, giving rise to large absorption factor [74]. Meanwhile, it was announced that SPPs play a negative role in *p* = 0 transmission [81]. From these two facts, evanescent waves in the negative diffraction order are strongly transmitted compared to propagating waves in the order 0, enabling sub-diffraction imaging.

### 2.5 Hyperlens

Another metamaterial-based lens enabling far-field sub-diffraction imaging is hyperlens. Hyperlenses are made of a hyperbolic metamaterial, a highly anisotropic material with hyperbolic dispersion. These materials have different signs of permittivity with regard to the directions. That is to say that permittivity in the parallel direction and perpendicular direction to the anisotropic axis has different sign. Such materials with anisotropic permittivity tensor act like metals in one direction and dielectrics in the other direction. Accordingly, from the dispersion relations in anisotropic medium, hyperbolic metamaterials have hyperboloid isofrequency surface, as can be seen in Fig. 1 (b) and (c). Due to this abnormal property, there have been many researches and it was discovered that hyperbolic metamaterials can realize enhancement in spontaneous emission, very large photonic density of states [38, 82–85], thermal engineering [86–88], and of course sub-diffraction imaging.

Here, *d* indicates thickness of each structure, the subscripts ⊥ and ∥ denote components perpendicular and parallel to the anisotropy axis, and the subscripts *m* and *d* indicate metal and dielectric material, respectively. Effective permittivity *ε*
_{∥} and *ε*
_{⊥} can be represented as functions of permittivity and thickness of metal and dielectric material. By tuning these parameters properly, hyperbolic dispersion can be achieved.

Hyperlens with tapered metallic nanowire array has been also studied numerically and experimentally [96–100], and resolution of one-fifteenth of a wavelength and magnification ratio of three were achieved numerically [99]. In this nanowires structure, sub-diffraction imaging is based on the excitation of the longitudinal resonance mode of the individual rods. Meanwhile, the sub-diffraction image reconstruction using multilayered hyperlenses relies on the excitation of the transverse resonance modes of SPPs. To understand the mechanism of hyperlens more specifically, let’s consider a cylindrical hyperlens with *ε*
_{
r
} < 0, *ε*
_{
θ
} > 0. Since it has an open isofrequency surface, arbitrarily large *k*
_{
θ
} with real *k*
_{
r
} is allowed in the lens. When evanescent waves enter the hyperlens, propagating modes of the lens are excited. In other words, evanescent waves are converted into propagating waves inside the hyperlens. During the propagation, *k*
_{
θ
}
*r* is a constant along the radial direction from the angular momentum conservation. *k*
_{
θ
} decreases as the wave propagates, so the sub-diffraction limited image is magnified by the factor of the outer radius divided by the inner radius. If *k*
_{
θ
} is compressed enough at the outer boundary so that *k*
_{
r
} becomes real value, evanescent waves becomes propagating waves at the outside of the hyperlens, enabling far-field propagation of the sub-diffraction information. Integrating with the conventional wide-field microscopes, the magnified resolution which is no more diffraction-limited can be captured by the regular objective lenses and CCD-cameras in real-time. Such benefits make hyperlenses more promising for the practical imaging solution.

In the cylindrical geometry proposed at the first time, super-resolution was allowed in only one direction and TM mode. Later, two full lateral dimensional sub-diffraction resolution was achieved by spherical shape of hyperlens with the unpolarized light at visible frequency, as shown in Fig. 8 (d) to (g) [94]. However, because both cylindrical and spherical geometry are not easy to position the object into the curved geometries, the concept of flat hyperlens was proposed. Hyperlens embedded in a metamaterial slab [101] and planar lenses using hyperbolic dispersion from metal-dielectric multilayered structure [102] was proposed as a solution. A flat hyperbolic metamaterial to which subwavelength grating is added was proved to be capable of far-field super-resolution imaging at visible frequency [103, 104].

Although a hyperlens provides far-field imaging, there are still some limitations. For example, an object has to be placed very close to the inner surface of the lens just like at the superlens. Hyperlens also suffers from high losses like superlens. Many researchers have tried to find hyperbolic metamaterial with lower losses, and as results, suggested to use active media [105, 106] and transparent conducting oxides (TCOs) to replace metals in near-IR range. Hyperbolic metamaterials composed of TCOs and dielectric exhibited low losses compared to the conventional metal-based ones [107, 108]. As a hyperlens becomes thicker, the image is more degraded due to the high absorption losses. However, a research proposed a hyperlens capable of sub-diffraction imaging at visible frequency with thickness as large as required. Using canalization, resolution of one-twentieth of the wavelength was confirmed [109].

For the high quality image, group velocity should remain a constant during the propagation. Since the group velocity is orthogonal to the dispersion curve, hyperlens with flat hyperbolic dispersion curve, which can be achieved by large negative *ε*
_{
r
} and small positive *ε*
_{
θ
}, is better. Another requirement of the undistorted image is an impedance matching condition, which indicates that a metal and a dielectric material should have similar order of polarization response. Since metals have real part of permittivity one order higher than that of dielectric materials, fill fraction of the metals has to be much smaller. It became a fabrication challenge, because grain structure of the thin film metal causes grain-boundary scattering for free electrons, lowering the image fidelity [110, 111]. Other factors responsible for losses are large reflection at the surface and scattering through the lens [112]. To reduce the surface reflection, studies about impedance-matched hyperlens was dedicated [113].

While hyperbolic metamaterials we have discussed so far are requiring difficult fabrication and suffering from high loss, hexagonal boron nitride, a natural hyperbolic material, has been emerged as a great alternative recently. Hyperbolic polaritons confined in a sub-diffractional volume were observed in a crystal of hexagonal boron nitride [114] and the sub-diffraction imaging lenses in IR frequency range were demonstrated [114–116]. Also, as alternatives to the hyperbolic materials with highly eccentric elliptic dispersion or extremely large refractive index (negative index is not necessary) works as well as hyperbolic metamaterials despite of the cut-off frequency in elliptic dispersion since the goal is supporting large *k*
_{
θ
} [117].

### 2.6 Metalens

The first one consists of a plasmonic metal-insulator-metal waveguide coupler (PWC) and a hyperbolic (or highly eccentric elliptic) metamaterial slab [118]. A plane wave can be focused to a point as it passes through a PWC and a metamaterial slab in order. When the incident plane wave excites the PWC, the waves with different transverse wavevectors and different phase transmit the metamaterial slab. By varying geometric parameters (width and height of the PWC), PWC can be designed so that the sum of phase gain from the metamaterial slab and from the PWC is a constant for every path. Under such a condition, plane waves interfere constructively at a point without loss of high spatial frequency waves thanks to unusual dispersion. Using this phase compensation mechanism, plane wave focusing and magnification are possible. Inversely, radiated beams from a point source are converted into a plane wave as they go through a metamaterial slab and a PWC. Without the PWC, a total internal reflection occurs when the waves with high wavevectors pass the exit surface of the lens, inhibiting the transmission of evanescent waves. But here, the PWC takes a role of bidirectional wavevector coupling and phase matching. The validity of the PWC-based metalens was demonstrated numerically [118].

The second type of metalens is metamaterial immersion lens (MIL) [119]. MILs have same phase compensation mechanism with a conventional lens; geometric shape of a MIL determines propagation length and hence, phase accumulation. Since diffraction phenomenon limits resolution to \( \frac{\uplambda}{2\mathrm{N}\mathrm{A}} \) where NA is a numerical aperture, it is important to make a lens with high NA. To achieve high NA, properly shaped high-index metamaterials were introduced. Interface of a MIL have to be designed to realize bidirectional coupling between the lens and air. By using a concave-shaped hyperbolic MIL where real part of permittivity along the propagating direction is negative, plane wave focusing was demonstrated. Whereas a convex shape is used to focus a plane wave for conventional materials, the hyperbolic MIL has concave surface due to negative refraction at the metamaterial-air interface [119]. One interesting thing is that the losses are important factors in the working mechanisms of MIL metalens. The waves with different transverse wavevectors suffer different amount of the loss due to their different loss coefficients, propagation length, and refraction angle. In a MIL, the waves with high transverse wavevectors attenuate less, and therefore, contribute more to construct an image, leading to high NA [119].

In a MIL, since the geometry is responsible for beam bending, the image quality is restricted by the geometrical and wave aberration. However, the conventional imaging devices with non-flat geometry can be compressed to the flat one using coordinate transformation because metamaterials are able to control light in almost arbitrary manners [122]. A flat metamaterial with gradually varying refractive index was proposed as an alternative metalens [120]. In the third metalens, a gradient-index (GRIN) metalens, spatially varying refractive index plays a role in bending light. A GRIN metalens is quite similar to a conventional GRIN lens, but the difference is that refractive profile is complicated in GRIN metalens while it is symmetric in the conventional one. A metalens consisting of patterned copper strips and an FR4 as a matrix in which refractive index is addressed by changing a proportion of the copper strips was proposed [123]. Since the copper strips are not resonant in the operation frequency, this metalens, or flattened Luneburg lens, exhibited low losses and broadband operation. Because artificial magnetic response is difficult to be fabricated, GRIN metalens in which permittivity distribution is designed in order to focus a plane wave was introduced and achieved a resolution of one-sixth of a wavelength [120]. A resolution of one-hundredth of a wavelength, and either wavelength- or incident angle- dependent focusing was numerically achieved by using metallic waveguide on which subwavelength patterns are non-periodically arranged [124]. A switchable GRIN metalens by shorting the gaps in SRRs were also presented [125].

Furthermore, other types of metalenses from the transformation optics approach have been proposed [126–129]. Planar metamaterial lenses which are capable of both plane waves focusing and magnifying sub-diffraction-limited objects have been studied [101, 122, 128, 129]. Restricted operating conditions of the planar metalens such as narrow bandwidth and directions of incident light were investigated and expanded by further research [130], but still remain as the major limitations.

### 2.7 Flat lens based on a metasurface

High losses, high fabrication cost, and complicated fabrication process have been pointed out as the main problems of plasmonic metamaterials [131, 132]. Plasmonic metamaterials with very thin thickness compared with the wavelength of the incident light are free from those disadvantages. These ultrathin planar metamaterials, called metasurfaces, can be also easily integrated with conventional optical devices due to their planar geometry.

While the convergence of optical waves relies on a gradual phase accumulation during the propagation in conventional lenses, focusing mechanism resulting from abrupt phase change can be achieved using phased array metasurfaces. Suppose meta-atoms, unit cells of a metasurface, are separated by a sub-wavelength distance and the interaction of the near-field is relatively small. When an oscillating electric field is applied to the metasurface, free electrons in meta-atoms oscillate forced by the electric field and restoring force. The strong interaction between incident light and the localized surface plasmons of meta-atoms is the key of the phase shift. Meta-atoms with spatially varying geometry work as resonators, giving rise to phase discontinuity through the sub-wavelength thickness [133, 134].

*θ*

_{ i },

*θ*

_{ t }, and

*θ*

_{ r }are the angles of incidence, refraction, and reflection, respectively,

*n*

_{ i }and

*n*

_{ t }are the refractive indices of the two media on the incidence and transmission side, respectively,

*k*

_{0}is a free-space wave number space, and ∇Φ is the gradient of phase along the interface. Equation (3) is for reflection and equation (4) is for refraction. The generalized Snell’s law, which is basically a momentum conservation equation, indicates that the direction of the refracted or reflected light (in this case, refracted light) can be controlled by assigning a proper phase gradient across the metasurface (Fig. 10 (a)). Namely, the phase-gradient metasurface can be designed to have a desired phase shift distribution by arranging properly-designed meta-atoms.

In an ideal phase-gradient metasurface, phase discontinuity strongly depends on the wavelength of incidence and geometry of the meta-atom, spanning all range from 0 to 2π. Beams that reach different position in metasurface refract with different angle as they pass through the metasurface in which meta-atoms with different geometry are arranged. When the image is reconstructed at a certain point by constructive interference of the refracted light, the metasurface functions as a lens. Since metasurfaces can control wavefront in nearly arbitrary manners, metasurfaces can be used in many applications. For example, they have been used to generate holograms, Gaussian beam, Bessel beams and optical vortex [144–147], and many researchers have shown that phase, amplitude, polarization state, frequency, momentum and angular momentum can be manipulated using metasurfaces [146, 148–150]. However, only metasurfaces related to imaging will be discussed in this review. It is also noted that the fundamental principles of the phase-gradient metasurface, which are related to the Pancharatnam-Berry phase [151], will not be discussed here.

The first demonstrated phase-gradient metasurface is shown in Fig. 10 (b) [144]. A unit cell of this nanoantenna-array (NA) metasurface is composed of eight symmetry breaking V-shaped nanoantennas with subwavelength size and separation. When an electromagnetic wave is applied, these V-antennas support two modes: symmetric modes and antisymmetric modes. Along the x-direction, two modes are excited with different phase and amplitude, resulting from the linear variation of the angle between the two rods of the antenna. The antennas with different geometry give rise to different phase shift. One-dimensional linear phase discontinuity results from the periodically patterned V-antennas. NA metasurface where nanoatennas are made of gold was analytically proved to enable 2π range of phase shift for cross-polarized light. [144] Not only V-shaped, but U- or C-shaped antennas were also used [152]. Modulation of phase, amplitude and polarization arising from two modes supported by V- and Y-shaped antennas was studied theoretically and experimentally [153].

Using phase shifting ability, planar lenses based on NA metasurface were presented. Aberration-free focusing using gold metasurface was experimentally demonstrated at THz region. Thin gold film on which V-shaped nanoantennas are radially distributed has hyperboloidal phase profile so that the scattered waves interfere constructively at the focal plane. These flat lenses exhibited high NA as well as zero monochromatic-aberration [145]. After that, metasurface-based lenses with complementary nanoantennas were proposed. A metasurface composed of array of complementary V-shaped antennas was fabricated in a gold film using photolithography and showed reduced noise due to directly transmitted light [154]. Another experimental research demonstrated a strong focusing ability of concentrically perforated gold films called a Babinet-inverted metalens. This metasurface accomplished a focal length of a few nanometers, high signal to noise ratio, and wavelength-controllable focal length by replacing plasmonic nano-antennas to nano-voids [155].

The phase shifting ability can be used to surpass the chromatic aberration, which is caused because light with different wavelength has different refractive angle. Recently, a metasurface based on dielectric resonators showed wavelength-dependent phase shift so that waves with three different wavelength deflect into the same angle [156]. In addition, metasurfaces acting as a lens in which either the incoming light converges or diverges depends on the helicity of the incidence were presented [157, 158]. When circularly polarized light enters the metasurfaces, the polarity is determined by the polarization of the light while the polarity of the conventional lenses are not interchangeable and thus, both magnification and demagnification are possible in the metasurface.

Although metasurfaces have showed new possibilities for imaging and further, manipulation and control of electromagnetic waves, they do not provide sub-diffraction imaging yet. Overcoming diffraction limit in imaging using flat lens based on metasurfaces remains as a future work.

### 2.8 Other lenses

- 1)
Acoustic metamaterial lens

- 2)
Magnetic metamaterial lens

*μ*

_{ r }= − 1 using surface coils can focus the radio frequency magnetic field, and therefore can be used in many applications such as magnetic resonance imaging (Fig. 11 (b)) [167] or wireless power transfer [168].

- 3)
Thermal metamaterial lens

As optical metamaterials transfer sub-diffraction optical information, the manipulation of nanoscale heat flux was realized by using metamaterials. It originates from the surface modes coupling which gives rise to a large near-field heat transfer modulation [169]. Furthermore, a multilayered composite material was proved to have abilities to shield, concentrate, and invert heat flux from its anisotropic characteristic (Fig. 11 (c)) [170]. Hyperbolic metasurfaces, very thin hyperbolic metamaterials, can also be used to control thermal radiation and near-field heat transfer, thanks to the diverging photonic density of state. Hence, controlling heat flow becomes possible, resulting in various applications including imaging, sensing, and detection [171].

## 3 Conclusion

In this review, we discussed how metamaterials have been used for better imaging surpassing and complementing the currently available optical microscopes. Metamaterials have shown ability to control electromagnetic wave at the nanoscale, allowing nanometers order of imaging resolution to come true. Over the past few decades, metamaterials with various designs and structures have been investigated for super-resolution imaging field to offer many different types of lenses which can overcome diffraction limit.

There are, however, some practical problems that hold real life applications. Although there have been intensive researches and tremendous efforts to achieve new science and technology, the major limitations of metamaterials – high losses, deep nanoscale fabrication issues, and narrow range of frequency, angle and polarization dependency, materials and size flexibilities, and integration with the conventional optics components- are still remained as future works. However, it is for sure that metamaterials have showed tremendous possibility and potential to change a paradigm in many fields, especially in optical imaging we discussed here. Therefore, with the development of nanofabrication and nanomanufacturing methods, and the integration of new creative ideas, overcoming the results and limitations mentioned in this review will be the continuous efforts to make metamaterial-based imaging techniques to be a next generation of imaging technology replacing current optical microscopy, which thus can be called nanoscopy.

## Declarations

### Acknowledgements

This work was supported by Focal Point Program (No. 2015-K1A3A1A16002157), Engineering Research Center program (No. 2011–0030075) and Pioneer Research Center program (No. 2015-M3C1A3022550) through the National Research Foundation of Korea (NRF) grant funded by the Ministry of Science, ICT and Future Planning (MSIP) of Korean government.

## Authors’ Affiliations

## References

- E Abbe, Beiträge zur Theorie des Mikroskops und der mikroskopischen Wahrnehmung. Arch. Mikroskop. Anat.
**9**(1), 413–418 (1873)View ArticleGoogle Scholar - MV Ardenne,
*U.K. Patent 511204-A*, 1938Google Scholar - R Reinhold,
*Patent DE 906737*, 1931Google Scholar - EH Synge, A suggested method for extending the microscopic resolution into the ultramicroscopic region. Phil. Mag
**6**, 356–362 (1928)View ArticleGoogle Scholar - EH Synge, An application of piezoelectricity to microscopy. Phil. Mag.
**13**, 297–300 (1932)View ArticleGoogle Scholar - U Dürig, DW Pohl, F Rohner, Near‐field optical‐scanning microscopy. J. Appl. Phys.
**59**, 3318–3327 (1986)View ArticleGoogle Scholar - Y Oshikane, T Kataoka, M Okuda, S Hara, H Inoue, M Nakano, Observation of nanostructure by scanning near-field optical microscope with small sphere probe. Sci. Technol. Adv. Mater.
**8**(3), 181–185 (2007)View ArticleGoogle Scholar - GK Bennig,
*US Patent 4724318 A*, 1988Google Scholar - G Binnig, CF Quate, C Gerber, Atomic Force Microscope. Phys. Rev. Lett.
**56**, 930–933 (1986)View ArticleGoogle Scholar - MJ Rust, M Bates, X Zhuang, Sub diffraction-limit imaging by stochastic optical reconstruction microscopy (STORM). Nature Methods
**3**(20), 793–796 (2006)View ArticleGoogle Scholar - E Betzig, GH Patterson, R Sougrat, OW Lindwasser, S Olenych, JS Bonifacino, MW Davidson, J Lippincott-Schwartz, HF Hess, Imaging Intracellular Fluorescent Proteins at Nanometer Resolution. Science
**313**(5793), 1642–1645 (2006)View ArticleGoogle Scholar - ST Hess, TP Giriajan, MD Mason, Ultra-high resolution imaging by Fluorescence Photoactivation Localization Microscopy. Biophysical Journal
**91**(11), 4258–4272 (2006)View ArticleGoogle Scholar - SW Hell, J Wichmann, Breaking the diffraction resolution limit by stimulated emission: stimulated-emission-depletion fluorescence microscopy. Opt. Lett
**19**, 780–782 (1994)View ArticleGoogle Scholar - E Rittweger, KY Han, SE Irvine, C Eggeling, SW Hell, STED microscopy reveals crystal colour centres with nanometric resolution. Nature Photon.
**3**, 144–147 (2009)View ArticleGoogle Scholar - MG Gustafsson, Nonlinear structured-illumination microscopy: Wide-field fluorescence imaging with theoretically unlimited resolution. Proc. Natl. Acad. Sci.
**102**(37), 13081–13086 (2005)View ArticleGoogle Scholar - MG Gustafsson, Surpassing the lateral resolution limit by a factor of two using structured illumination microscopy. Journal of Microscopy
**198**, 82–87 (2000)View ArticleGoogle Scholar - B Huang, H Babcock, X Zhuang, Breaking the diffraction barrier: super-resolution imaging of cells. Cell
**143**, 1047–1058 (2010)View ArticleGoogle Scholar - BC Tom, AK Katsaggelos, NP Galatsanos, Reconstruction of a high resolution image from registration and restoration of low resolution images. Proceedings of IEEE International Conference on Image Processing
**3**, 553–557 (1994)View ArticleGoogle Scholar - VG Veselago, The electrodynamics of substances with simultaneously negative values of ε and μ. Sov. Phys. Uspekhi
**10**, 509–514 (1968)View ArticleGoogle Scholar - DR Smith, WJ Padilla, DC Vier, SC Nemat-Nasser, S Schultz, Composite medium with simultaneously negative permeability and permittivity. Phys. Rev. Lett.
**84**(18), 4184–4187 (2000)View ArticleGoogle Scholar - RA Shelby, DR Smith, S Schultz, Experimental Verification of a Negative Index of Refraction. Science
**292**(5514), 77–79 (2001)View ArticleGoogle Scholar - RA Shelby, DR Smith, SC Nemat-Nasser, S Schultz, Microwave transmission through a two-dimensional, isotropic, left-handed metamaterial. Appl. Phys. Lett.
**78**(4), 489–491 (2001)View ArticleGoogle Scholar - YJ Hsu, YC Huang, JS Lih, JL Chern, Electromagnetic resonance in deformed split ring resonators of left-handed meta-materials. J. Appl. Phys.
**96**(4), 1979–1982 (2004)View ArticleGoogle Scholar - AA Houck, JB Brock, IL Chuang, Experimental Observations of a Left-Handed Material That Obeys Snell’s Law. Phys. Rev. Lett
**90**, 137401 (2003)View ArticleGoogle Scholar - A Grbic, GV Eleftheriades, Overcoming the Diffraction Limit with a Planar Left-Handed Transmission-Line Lens. Phys. Rev. Lett
**92**(11), 117403 (2004)View ArticleGoogle Scholar - J Valentine, S Zhang, T Zentgraf, E Ulin-Aila, DA Genov, G Bartel, X Zhang, Three-dimensional optical metamaterial with a negative refractive index. Nature
**455**, 376–379 (2008)View ArticleGoogle Scholar - S Zhang, YS Park, J Li, X Lu, W Zhang, X Zhang, Negative Refractive Index in Chiral Metamaterials. Phys. Rev. Lett.
**102**, 023901 (2009)View ArticleGoogle Scholar - JB Pendry, A Chiral, Route to Negative Refraction. Science
**306**(5), 1353–1355 (2004)View ArticleGoogle Scholar - CG Parazzoli, RB Greegor, K Li, BEC Koltenbah, M Tanielian, Experimental verification and simulation of negative index of refraction using Snell’s law. Phys. Rev. Lett
**90**, 107401 (2003)View ArticleGoogle Scholar - VM Shalaev, W Cai, UK Chettiar, HK Yuan, AK Sarychev, VP Drachev, AV Kildishev, Negative index of refraction in optical metamaterials. Opt. Lett.
**30**(24), 3356–3358 (2005)View ArticleGoogle Scholar - S Zhang, W Fan, NC Panoiu, KJ Malloy, RM Osgood, SRJ Brueck, Experimental demonstration of near-infrared negative-index metamaterials. Phys. Rev. Lett.
**95**, 137404 (2005)View ArticleGoogle Scholar - G Dolling, C Enkrich, M Wegener, CM Soukoulis, S Linden, Simultaneous negative phase and group velocity of light in a metamaterial. Science
**312**(5775), 892–894 (2006)View ArticleGoogle Scholar - J Yao, Z Liu, Y Liu, Y Wang, C Sun, G Bartal, AM Stacy, X Zhang, Optical negative refraction in bulk metamaterials of nanowires. Science
**321**(5891), 930–930 (2008)View ArticleGoogle Scholar - SP Burgos, R de Waele, A Polman, HA Atwater, A single-layer wide-angle negative-index metamaterial at visible frequencies. Nature Mater
**9**, 407–412 (2010)View ArticleGoogle Scholar - HJ Lezec, JA Dionne, HA Atwater, Negative refraction at visible frequencies. Science
**316**(5823), 430–432 (2007)View ArticleGoogle Scholar - E Verhagen, R de Waele, L Kuipers, A Polman, Three-dimensional negative index of refraction at optical frequencies by coupling plasmonic waveguides. Phys. Rev. Lett.
**105**(22), 223901 (2010)View ArticleGoogle Scholar - JB Pendry, A Holden, D Robbins, W Stewart, Magnetism from conductors and enhanced nonlinear phenomena. IEEE Trans. Microwave Theory and Techniques
**47**(11), 2075–2084 (1999)View ArticleGoogle Scholar - Z Jacob, JY Kim, GV Naik, A Boltasseva, EE Narimanov, VM Shalaev, Engineering photonic density of states using metamaterials. Appl. Phys. B
**100**(1), 215–218 (2010)View ArticleGoogle Scholar - JB Pendry, D Schurig, DR Smith, Controlling electromagnetic fields. Science
**312**(5781), 1780–1782 (2006)View ArticleGoogle Scholar - A Greenleaf, Y Kurylev, M Lassas, G Uhlmann, Cloaking devices, electromagnetic wormholes, and transformation optics. SIAM Rev.
**51**(1), 3–33 (2009)View ArticleGoogle Scholar - JB Pendry, Negative Refraction Makes a Perfect Lens. Phys. Rev. Lett.
**85**(18), 3966–3969 (2000)View ArticleGoogle Scholar - JB Pendry, Negative refraction. Contemporary Physics
**45**(3), 191–202 (2004)View ArticleGoogle Scholar - N Garcia, M Nieto-Vesperinas, Left-Handed Materials Do Not Make a Perfect Lens. Phys. Rev. Lett
**88**(20), 207403-1-4 (2002)View ArticleGoogle Scholar - JB Pendry, Comment on “Left-Handed Materials Do Not Make a Perfect Lens”. Phys. Rev. Lett
**91**(9), 099701 (2003)View ArticleGoogle Scholar - G Gómez-Santos, Universal Features of the Time Evolution of Evanescent Modes in a Left-Handed Perfect Lens. Phys. Rev. Lett
**90**(7), 077401 (2003)View ArticleGoogle Scholar - DR Smith, D Schurig, M Rosenbluth, S Schultz, Limitations on subdiffraction imaging with a negative refractive index slab. Appl. Phys. Lett.
**82**(10), 1506–1508 (2003)View ArticleGoogle Scholar - SA Ramakrishna, JB Pendry, D Schurig, DR Smith, S Schultz, The asymmetric lossy near-perfect lens. Journal of Modern Optics
**49**(10), 1747–1762 (2002)View ArticleGoogle Scholar - ZW Liu, N Fang, TJ Yen, X Zhang, Rapid growth of evanescent wave by a silver superlens. Appl. Phys. Lett.
**83**(25), 5184–5186 (2003)View ArticleGoogle Scholar - N Fang, ZW Liu, TJ Yen, X Zhang, Regenerating evanescent waves from a silver superlens. Opt. Express
**11**(7), 682–687 (2003)View ArticleGoogle Scholar - A Giannattasio, IR Hooper, WL Barnes, Transmission of light through thin silver film via surface plasmon-polaritons. Opt. Express
**12**(24), 5881–5886 (2004)View ArticleGoogle Scholar - X Zhang, Z Liu, Superlenses to overcome the diffraction limit. Nature Mater.
**7**(6), 435–441 (2008)View ArticleGoogle Scholar - N Fang, H Lee, C Sun, X Zhang, Sub-Diffraction-Limited Optical Imaging with a Silver Superlens. Science
**308**(5721), 534–537 (2005)View ArticleGoogle Scholar - RJ Blaikie, DOS Melville, Imaging through planar silver lenses in the optical near field. J. Opt. A: Pure Appl. Opt
**7**, S176–S183 (2005)View ArticleGoogle Scholar - DOS Melville, RJ Blaikie, Near-field optical lithography using a planar silver lens. J. Vac. Sci. Technol. B
**22**(6), 3470–3474 (2004)View ArticleGoogle Scholar - N Fang, X Zhang, Imaging properties of a metamaterial superlens. Appl. Phys. Lett.
**82**(2), 161–163 (2003)View ArticleGoogle Scholar - T Taubner, D Korobkin, Y Urzhumov, G Shvets, R Hillenbrand, Near-Field Microscopy Through a SiC Superlens. Science
**313**(5793), 1595–1595 (2006)View ArticleGoogle Scholar - M Jablan, H Buljan, M Soljačić, Plasmonics in graphene at infrared frequencies. Phys. Rev. B
**80**, 245435 (2009)View ArticleGoogle Scholar - P Tassin, T Koschny, M Kafesaki, CM Soukoulis, A comparison of graphene, superconductors and metals as conductors for metamaterials and plasmonics. Nature Photon.
**6**, 259–264 (2012)View ArticleGoogle Scholar - JB Khurgin, G Sun, In search of the elusive lossless metal. Appl. Phys. Lett
**96**(18), 181102 (2010)View ArticleGoogle Scholar - SA Ramakrishna, JB Pendry, Removal of absorption and increase in resolution in a near-field lens via optical gain. Phys. Rev. B
**67**, 201101 (2003)View ArticleGoogle Scholar - MG Blaber, MD Arnold, MJ Ford, A review of the optical properties of alloys and intermetallics for plasmonics. J. Phys.: Condens. Matter
**22**, 143201 (2010)Google Scholar - GV Naik, J Kim, A Boltasseva, Oxides and nitrides as alternative plasmonic materials in the optical range [Invited]. Opt. Mater. Express
**1**(6), 1090–1099 (2011)View ArticleGoogle Scholar - AJ Hoffman, LV Alekseyev, SS Howard, KJ Franz, D Wasserman, VA Podolskiy, EE Narimanov, DL Sivco, C Gmachl, Negative refraction in semiconductor metamaterials. Nature Mater
**6**, 946–950 (2007)View ArticleGoogle Scholar - GV Naik, A Boltasseva, Semiconductors for plasmonics and metamaterials. Phys. Status Solidi RRL
**4**(10), 295–297 (2010)View ArticleGoogle Scholar - CJ Regan, D Dominguez, LG de Peralta, AA Bernussi, Far-field optical superlenses without metal. Appl. Phys. Lett
**113**, 183105 (2013)Google Scholar - H Lee, Y Xiong, N Fang, W Srituravanich, S Durant, M Ambati, C Sun, X Zhang, Realization of optical superlens imaging below the diffraction limit. New J. Phys.
**7**, 255 (2005)View ArticleGoogle Scholar - E Shamonina, V Kalinin, K Ringhofer, L Solymar, Imaging, compression and Poynting vector streamlines for negative permittivity mateirals. Electron. Lett.
**37**, 1243–1244 (2001)View ArticleGoogle Scholar - SA Ramakrishna, JB Pendry, MCK Wiltshire, WJ Stewart, Imaging the near field. J. Mod. Opt.
**50**(9), 1419–1430 (2003)View ArticleGoogle Scholar - SC Kehr, YM Liu, LW Martin, P Yu, M Gajek, SY Yang, CH Yang, MT Wenzel, R Jacob, HG von Ribbeck, M Helm, X Zhang, LM Eng, R Ramesh, Near-field examination of perovskite-based superlenses and superlens-enhanced probe-object coupling. Nature Commun.
**2**, 249 (2011)View ArticleGoogle Scholar - M Fehrenbacher, S Winnerl, H Schneider, J Doring, SC Kehr, LM Eng, Y Huo, OG Schmidt, K Yao, Y Liu, M Helm, Plasmonic superlensing in doped GaAs. Nano Lett.
**15**(2), 1057–1061 (2015)View ArticleGoogle Scholar - P Li, T Wang, H Bockmann, T Taubner, Graphene-Enhanced Infrared Near-Field Microscopy. Nano Lett.
**14**(8), 4400–4405 (2014)View ArticleGoogle Scholar - P Li, T Taubner, Multi-wavelength superlensing with layered phonon-resonant dielectrics. Opt. Express
**20**(11), 11787–11795 (2012)View ArticleGoogle Scholar - S Durant, Z Liu, N Fang, X Zhang, Theory of optical imaging beyond the diffraction limit with a far-field superlens. Proc. SPIE 6323, Plasmonics: Metallic Nanostructures and their Optical Properties
**IV**, 63231H (2006)Google Scholar - S Durant, Z Liu, JM Steele, X Zhang, Theory of the transmission properties of an optical far-field superlens for imaging beyond the diffraction limit. J. Opt. Soc. Am. B
**23**(11), 2383–2392 (2006)View ArticleGoogle Scholar - Z Liu, S Durant, H Lee, Y Pikus, N Fang, Y Xiong, C Sun, X Zhang, Far-Field Optical Superlens. Nano Lett.
**7**(2), 403–408 (2007)View ArticleGoogle Scholar - Z Liu, S Durant, H Lee, Y Pikus, Y Xiong, C Sun, X Zhang, Experimental studies of far-field superlens for sub-diffractional optical imaging. Opt. Express
**15**(11), 6947–6954 (2007)View ArticleGoogle Scholar - Z Liu, S Durant, H Lee, Y Xiong, Y Pikus, C Sun, X Zhang, Near-field Moire effect mediated by surface plasmon polariton excitation. Opt. Lett.
**32**(6), 629–631 (2007)View ArticleGoogle Scholar - O Kafri, I Glatt,
*The Physics of Moiré Metrology*(Wiley, New York, 1989), p. 4Google Scholar - V Krishnamurthi, B Bailey, F Lanni, Image processing in 3-D standing-wave fluorescence microscopy. Proc. SPIE Int. Soc. Opt. Eng.
**2655**, 18–25 (1996)Google Scholar - Y Xiong, Z Liu, S Durant, H Lee, C Sun, X Zhang, Tuning the far-field superlens: from UV to visible. Opt. Express
**15**(12), 7095–7102 (2007)View ArticleGoogle Scholar - Q Cao, P Lalanne, Negative Role of Surface Plasmons in the Transmission of Metallic Gratings with Very Narrow Slits. Phys. Rev. Lett.
**88**, 057403 (2002)View ArticleGoogle Scholar - X Yang, J Yao, J Rho, X Yin, X Zhang, Experimental realization of three-dimensional indefinite cavities at the nanoscale with anomalous scaling laws. Nature Photon.
**6**, 450–454 (2012)View ArticleGoogle Scholar - D Lu, JJ Kan, EE Fullerton, Z Liu, Enhancing spontaneous emission rates of molecules using nanopatterned multilayer hyperbolic metamaterials. Nat. Nanotechnol.
**9**(1), 48–53 (2014)View ArticleGoogle Scholar - Z Jacob, I Smolyaninov, EE Narimanov, Broadband Purcell effect: Radiative decay engineering with metamaterials. Appl. Phys. Lett.
**100**(18), 181105–181114 (2009)View ArticleGoogle Scholar - MA Noginov, H Li, YA Barnakov, D Dryden, G Nataraj, G Zhu, CE Bonner, M Mayy, Z Jacob, EE Narimanov, Controlling spontaneous emission with metamaterials. Opt. Lett.
**35**(11), 1863–1865 (2010)View ArticleGoogle Scholar - Z Yu, NP Sergeant, T Skauli, G Zhang, H Wang, S Fan, Enhancing far-field thermal emission with thermal extraction. Nat. Commun.
**4**, 1730 (2013)View ArticleGoogle Scholar - Y Guo, CL Cortes, S Molesky, Z Jacob, Broadband super-Planckian thermal emission from hyperbolic metamaterials. Appl. Phys. Lett.
**101**, 131106 (2012)View ArticleGoogle Scholar - EE Narimanov, II Smolyaninov, Beyond Stefan-Boltzmann Law: Thermal Hyper-Conductivity, in
*Quantum Electronics and Laser Science Conference, San Jose*, 2012Google Scholar - Z Jacob, LV Alekseyev, EE Narimanov, Optical hyperlens: far-field imaging beyond the diffraction limit. Opt. Express
**14**(18), 8247–8256 (2006)View ArticleGoogle Scholar - A Salandrino, N Engheta, Far-field subdiffraction optical microscopy using metamaterial crystals: theory and simulations. Phys. Rev. B
**74**, 075103 (2006)View ArticleGoogle Scholar - B Wood, JB Pendry, Directed Sub-Wavelength Imaging Using a Layered Metal-Dielectric System. Phys. Rev. B
**74**, 115116 (2006)View ArticleGoogle Scholar - Z Liu, H Lee, Y Xiong, C Sun, X Zhang, Far-field optical hyperlens magnifying sub-diffraction-limited objects. Science
**315**(5819), 1686–1686 (2007)View ArticleGoogle Scholar - H Lee, Z Liu, Y Xiong, C Sun, X Zhang, Development of optical hyperlens for imaging below the diffraction limit. Opt. Express
**15**(24), 15886–15891 (2007)View ArticleGoogle Scholar - J Rho, Z Ye, Y Xiong, X Yin, Z Liu, H Choi, G Bartal, X Zhang, Spherical hyperlens for two-dimensional sub-diffractional imaging at visible frequencies. Nature Commun.
**1**, 143 (2010)View ArticleGoogle Scholar - II Smolyaninov, YJ Hung, CC Davis, Magnifying superlens in the visible frequency range. Science
**315**(5819), 1699–1701 (2007)View ArticleGoogle Scholar - G Shvets, S Trendafilov, JB Pendry, A Sarychev, Guiding, focusing, and sensing on the subwavelength scale using metallic wire arrays. Phys. Rev. Lett.
**99**, 053903 (2007)View ArticleGoogle Scholar - A Ono, J Kato, S Kawata, Subwavelength optical imaging through a metallic nanorod array. Phys. Rev. Lett.
**95**(26), 267407 (2005)View ArticleGoogle Scholar - P Ikonen, C Simovski, S Tretyakov, P Belov, Y Hao, Magnification of subwavelength field distributions at microwave frequencies using a wire medium slab operating in the canalization regime. Appl. Phys. Lett.
**91**, 104102 (2007)View ArticleGoogle Scholar - Y Zhao, G Palikaras, PA Belov, RF Dubrovka, C Simovski, Y Hao, CG Parini, Magnification of subwavelength field distributions using a tapered array of metallic wires with planar interfaces and an embedded dielectric phase compensator. New J. Phys.
**12**, 103045 (2010)View ArticleGoogle Scholar - S Kawata, A Ono, P Verma, Subwavelength colour imaging with a metallic nanolens. Nature Photon.
**2**(7), 438–442 (2008)View ArticleGoogle Scholar - AV Kildishev, VM Shalaev, Engineering space for light via transformation optics. Opt. Lett.
**33**(1), 43–45 (2008)View ArticleGoogle Scholar - W Wang, H Xing, L Fang, Y Liu, J Ma, L Lin, C Wang, X Luo, Far-field imaging device: planar hyperlens with magnification using multi-layer metamaterial. Opt. Express
**16**(25), 21142–21148 (2008)View ArticleGoogle Scholar - Y Xiong, Z Liu, C Sun, X Zhang, Two-Dimensional Imaging by Far-Field Superlens at Visible Wavelengths. Nano Letters
**7**(11), 3360–3365 (2007)View ArticleGoogle Scholar - S Thongrattanasiri, VA Podolskiy, Hyper-gratings: nanophotonics in planar anisotropic metamaterials. Opt. Lett.
**34**(7), 890–892 (2009)View ArticleGoogle Scholar - MA Vincenti, D de Ceglia, V Rondinone, A Ladisa, A D’Orazio, MJ Bloemer, M Scalora, Loss compensation in metal-dielectric structures in negative-refraction and super-resolving regimes. Phys. Rev. A
**80**, 053807 (2009)View ArticleGoogle Scholar - X Ni, S Ishii, MD Thoreson, VM Shalaev, S Han, S Lee, AV Kildishev, Loss-compensated and active hyperbolic metamaterials. Opt. Express
**19**(25), 25242–25254 (2011)View ArticleGoogle Scholar - GV Naik, J Liu, AV Kildishev, VM Shalaev, A Boltasseva, Demonstration of Al:ZnO as a plasmonic component for near-infrared metamaterials. Proc. Natl. Acad. Sci.
**109**(23), 8834–8838 (2012)View ArticleGoogle Scholar - GV Naik, VM Shalaev, A Boltasseva, Alternative Plasmonic Materials: Beyond Gold and Silver. Adv. Mater.
**25**(24), 3264–3294 (2013)View ArticleGoogle Scholar - PA Belov, Y Hao, Subwavelength imaging at optical frequencies using a transmission device formed by a periodic layered metal-dielectric structure operating in the canalization regime. Phys. Rev. B
**73**, 113110 (2006)View ArticleGoogle Scholar - F Warkusz, Electrical and mechanical properties of thin metal films: Size effects. Prog. Surf. Sci
**10**(3), 287–382 (1980)View ArticleGoogle Scholar - K Fuchs, The conductivity of thin metallic films according to the electron theory of metals. Math. Proc. Cambridge Philos. Soc
**34**(10), 100–108 (1938)View ArticleGoogle Scholar - Z Jacob, LV Alekseyev, EE Narimanov, Semiclassical theory of the hyperlens. J. Opt. Soc. Am. A
**24**(10), A52–A59 (2007)View ArticleGoogle Scholar - AV Kildishev, EE Narimanov, Impedance-matched hyperlens. Opt. Lett.
**32**(23), 3432–3434 (2007)View ArticleGoogle Scholar - JD Caldwell, AV Kretinin, Y Chen, V Giannini, MM Fogler, Y Francescato, CT Ellis, JG Tischler, CR Woods, AJ Giles, M Hong, K Watanabe, T Taniguchi, SA Maier, KS Novoselov, Sub-diffractional volume-confined polaritons in the natural hyperbolic material hexagonal boron nitride. Nature Commun
**5**, 5221 (2014)View ArticleGoogle Scholar - S Dai, Q Ma, T Andersen, AS Mcleod, Z Fei, MK Liu, M Wagner, K Watanabe, T Taniguchi, M Thiemens, F Keilmann, P Jarillo-Herrero, MM Fogler, DN Basov, Subdiffractional focusing and guiding of polaritonic rays in a natural hyperbolic material. Nature Commun.
**6**, 6963 (2015)View ArticleGoogle Scholar - P Li, M Lewin, AV Kretinin, JD Caldwell, KS Novoselov, T Taniguchi, K Watanabe, F Gaussmann, T Taubner, Hyperbolic phonon-polaritons in boron nitride for near-field optical imaging. arXiv:1502.04093v2Google Scholar
- C Ma, R Aguinaldo, Z Liu, Advances in the hyperlens. Chin. Sci. Bull.
**55**(24), 2618–2624 (2010)View ArticleGoogle Scholar - C Ma, Z Liu, A super resolution metalens with phase compensation mechanism. Appl. Phys. Lett
**96**(18), 183103 (2010)View ArticleGoogle Scholar - C Ma, Z Liu, Focusing light into deep subwavelength using metamaterial immersion lenses. Opt. Express
**18**(5), 4838–4844 (2010)View ArticleGoogle Scholar - C Ma, MA Escobar, Z Liu, Extraordinary light focusing and Fourier transform properties of gradient-index metalenses. Phys. Rev. B
**84**, 195142 (2011)View ArticleGoogle Scholar - D Lu, Z Liu, Hyperlenses and metalenses for far-field super-resolution imaging. Nature Commun.
**3**, 1205 (2012)Google Scholar - DA Roberts, N Kundtz, DR Smith, Optical lens compression via transformation optics. Opt. Express
**17**(19), 16535–16542 (2009)View ArticleGoogle Scholar - N Kundtz, DR Smith, Extreme-angle broadband metamaterial lens. Nature Mater.
**9**(2), 129–132 (2010)View ArticleGoogle Scholar - L Verslegers, PB Catrysse, Z Yu, S Fan, Deep-Subwavelength Focusing and Steering of Light in an Aperiodic Metallic Waveguide Array. Phys. Rev. Lett.
**103**, 033902 (2009)View ArticleGoogle Scholar - IE Khodasevych, IV Shadrivov, DA Powell, WST Rowe, A Mitchell, Pneumatically switchable graded index metamaterial lens. Appl. Phys. Lett
**102**(3), 031904 (2013)View ArticleGoogle Scholar - DH Kwon, DH Werner, Transformation optical designs for wave collimators, flat lenses and right-angle bends. New J. Phys
**10**, 115023 (2008)View ArticleGoogle Scholar - R Yang, W Tang, Y Hao, A broadband zone plate lens from transformation optics. Opt. Express
**19**(13), 12348–12355 (2011)View ArticleGoogle Scholar - S Han, Y Xiong, D Genov, Z Liu, G Bartel, X Zhang, Ray optics at a deep-subwavelength scale: a transformation optics approach. Nano Lett.
**8**(12), 4243–4247 (2008)View ArticleGoogle Scholar - M Tsang, D Psaltis, Magnifying perfect lens and superlens design by coordinate transformation. Phys. Rev. B
**77**, 035122 (2008)View ArticleGoogle Scholar - ZH Jiang, MD Gregory, DH Werner, Experimental demonstration of a broadband transformation optics lens for highly directive multibeam emission. Phys. Rev. B
**84**, 165111 (2011)View ArticleGoogle Scholar - A Boltasseva, HA Atwater, Low-loss plasmonic metamaterials. Science
**331**(6015), 290–291 (2011)View ArticleGoogle Scholar - CM Soukoulis, M Wegener, Past achievements and future challenges in the development of three-dimensional photonic metamaterials. Nature Photon
**5**, 523–530 (2011)Google Scholar - N Meinzer, WL Barnes, IR Hooper, Plasmonic meta-atoms and metasurfaces. Nature Photon.
**8**(12), 889–898 (2014)View ArticleGoogle Scholar - N Yu, F Capasso, Flat optics with designer metasurfaces. Nature Mater.
**13**(2), 139–150 (2014)View ArticleGoogle Scholar - DM Pozar, SD Targonski, HD Syrigos, Design of millimeter wave microstrip reflectarrays. IEEE Trans. Antennas Propag.
**45**(2), 287–296 (1997)View ArticleGoogle Scholar - JA Encinar, Design of two-layer printed reflectarrays using patches of variable size. IEEE Trans. Antennas Propag.
**49**(10), 1403–1410 (2001)View ArticleGoogle Scholar - DT McGrath, Planar three-dimensional constrained lenses. IEEE Trans. Antennas Propag.
**34**(1), 46–50 (1986)View ArticleGoogle Scholar - DM Pozar, Flat lens antenna concept using aperture coupled microstrip patches. Electron. Lett.
**32**, 2109–2111 (1996)View ArticleGoogle Scholar - P Padilla, A Muñoz-Acevedo, M Sierra-Castañer, M Sierra-Pérez, Electronically reconfigurable transmitarray at Ku band for microwave applications. IEEE Trans. Antennas Propag.
**58**(8), 2571–2579 (2010)View ArticleGoogle Scholar - L Verslegers, PB Catrysse, Z Yu, JS White, ES Barnard, ML Brongersma, S Fan, Planar Lenses Based on Nanoscale Slit Arrays in a Metallic Film. Nano Lett.
**9**(1), 235–238 (2009)View ArticleGoogle Scholar - FM Huang, TS Kao, VA Fedotoc, Y Chen, N Zheludev, Nanohole array as a lens. Nano Lett.
**8**(8), 2469–2472 (2008)View ArticleGoogle Scholar - FM Huang, N Zheludev, Super-Resolution without Evanescent Waves. Nano Lett.
**9**(3), 1249–1254 (2009)View ArticleGoogle Scholar - ETF Rogers, J Lindberg, T Roy, S Savo, JE Chad, MR Dennis, NI Zheludev, A super-oscillatory lens optical microscope for subwavelength imaging. Nature Mater
**11**, 432–435 (2012)View ArticleGoogle Scholar - N Yu, P Genevet, MA Kats, F Aieta, JP Tetienne, F Capasso, Z Gaburro, Light propagation with phase discontinuities: generalized laws of reflection and refraction. Science
**334**(6054), 333–337 (2011)View ArticleGoogle Scholar - F Aieta, P Genevet, MA Kats, N Yu, R Blanchard, Z Gaburro, F Capasso, Aberration-free ultrathin flat lenses and axicons at telecom wavelengths based on plasmonic metasurfaces. Nano Lett.
**12**(9), 4932–4936 (2012)View ArticleGoogle Scholar - P Genevet, N Yu, F Aieta, J Lin, MA Kats, R Blanchard, MO Scully, Z Gaburro, F Capasso, Ultra-thin plasmonic optical vortex plate based on phase discontinuities. Appl. Phys. Lett.
**100**, 013101 (2012)View ArticleGoogle Scholar - L Huang, X Chen, H Mühlenbernd, H Zhang, S Chen, B Bai, Q Tan, G Jin, KW Cheah, CW Qiu, J Li, T Zentgraf, S Zhang, Three-dimensional optical holography using a plasmonic metasurface. Nature Commun.
**4**, 28 (2013). Semiconductors for plasmonics and metamaterials 08Google Scholar - F Aieta, P Genevet, N Yu, MA Kats, Z Gaburro, F Capasso, Out-of-plane reflection and refraction of light by anisotropic optical antenna metasurfaces with phase discontinuities. Nano Lett.
**12**(3), 1702–1706 (2012)View ArticleGoogle Scholar - R Blanchard, G Aoust, P Genevet, N Yu, MA Kats, Z Gaburro, F Capasso, Modeling nanoscale V-shaped antennas for the design of optical phased arrays. Phys. Rev. B
**85**, 155457 (2012)View ArticleGoogle Scholar - S Larouche, DR Smith, Reconciliation of generalized refraction with diffraction theory. Opt. Lett.
**37**(12), 2391–2393 (2012)View ArticleGoogle Scholar - E Hasman, V Kleiner, G Biener, A Niv, Polarization dependent focusing lens by use of quantized Pancharatnam–Berry phase diffractive optics. Appl. Phys. Lett.
**82**(3), 328–330 (2003)View ArticleGoogle Scholar - L Liu, Z Zhang, M Kenney, X Su, N Xu, C Ouyang, Y Shi, J Han, W Zhang, S Zhang, Broadband metasurfaces with simultaneous control of phase and amplitude. Adv. Mater.
**26**(29), 5031–5036 (2014)View ArticleGoogle Scholar - MA Kats, P Genevet, G Aoust, NF Yu, R Blanchard, F Aieta, Z Gaburro, F Capasso, Giant birefringence in optical antenna arrays with widely tailorable optical anisotropy. Proc. Natl. Acad. Sci.
**109**, 12364–12368 (2012)View ArticleGoogle Scholar - D Hu, X Wang, S Feng, J Ye, W Sun, Q Kan, PJ Klar, Y Zhang, Ultrathin terahertz planar lenses. Adv. Opt. Mater.
**1**(2), 186–191 (2013)View ArticleGoogle Scholar - X Ni, S Ishii, AV Kildishev, VM Shalaev, Ultra-thin, planar, Babinet-inverted plasmonic metalenses. Light: Science & Applications
**2**(4), e72 (2013)View ArticleGoogle Scholar - F Aieta, MA Kats, P Genevet, F Cappaso, Multiwavelength Achromatic Metasurfaces by Dispersive Phase Compensation. Science
**347**(6228), 1342–1345 (2015)View ArticleGoogle Scholar - X Chen, L Huang, H Muhlenbernd, G Li, B Bai, Q Tan, G Jin, CW Qiu, S Zhang, T Zentgraf, Dual-polarity plasmonic metalens for visible light. Nature Commun.
**3**, 1198 (2012)View ArticleGoogle Scholar - X Chen, L Huang, H Muhlenbernd, G Li, B Bai, Q Tan, G Jin, CW Qiu, T Zentgraf, S Zhang, Reversible Three Dimensional Focusing of Visible Light with Ultrathin Plasmonic Flat Lens. Adv. Opt. Mater.
**1**(7), 517–521 (2013)View ArticleGoogle Scholar - F Cervera, L Sanchis, JV Sánchez-Pérez, R Martínez-Sala, C Rubio, F Meseguer, C López, D Caballero, J Sánchez-Dehesa, Refractive acoustic devices for airborne sound. Phys. Rev. Lett.
**88**, 023902 (2001)View ArticleGoogle Scholar - M Ke, Z Liu, Z Cheng, J Li, P Peng, J Shi, Flat superlens by using negative refraction in two-dimensional phononic crystals. Solid State Commun.
**142**(3), 177–180 (2007)View ArticleGoogle Scholar - J Liu, CT Chan, Double-negative acoustic metamaterial. Phys. Rev. E
**70**, 055602(R) (2004)View ArticleGoogle Scholar - N Fang, D Xi, J Xu, M Ambati, W Srituravanich, C Sun, X Zhang, Ultrasonic metamaterials with negative modulus. Nature Mater.
**5**, 452–456 (2006)View ArticleGoogle Scholar - S Zhang, L Yin, N Fang, Focusing ultrasound with an acoustic metamaterial network. Phys. Rev. Lett.
**102**, 194301 (2009)View ArticleGoogle Scholar - S Guenneau, A Movchan, G Pétursson SA, Ramakrishna. Acoustic metamaterials for sound focusing and confinement. New J. Phys
**9**, 399 (2007)View ArticleGoogle Scholar - X Ao, CT Chan, Far-field image magnification for acoustic waves using anisotropic acoustic metamaterials. Phys. Rev. E
**77**, 025601(R) (2008)View ArticleGoogle Scholar - J Li, L Fok, X Yin, G Bartal, X Zhang, Experimental demonstration of an acoustic magnifying hyperlens. Nature Mater
**8**, 931–934 (2009)View ArticleGoogle Scholar - MJ Freire, R Marqués, L Jelinek, Experimental demonstration of a μ = −1 metamaterial lens for magnetic resonance imaging. Appl. Phys. Lett
**93**, 231108 (2008)View ArticleGoogle Scholar - G Lipworth, J Ensworth, K Seetharam, D Huang, JS Lee, P Schmalenberg, T Nomura, MS Reynolds, DR Smith, Y Urzhumov, Magnetic Metamaterial Superlens for Increased Range Wireless Power Transfer. Sci. Rep.
**4**, 3642 (2014)View ArticleGoogle Scholar - L Cui, Y Huang, J Wang, KY Zhu, Ultrafast modulation of near-field heat transfer with tunable metamaterials. Appl. Phys. Lett.
**102**(5), 053106 (2013)View ArticleGoogle Scholar - S Narayana, Y Sato, Heat Flux Manipulation with Engineered Thermal Materials. Phys. Rev. Lett.
**108**, 214303 (2012)View ArticleGoogle Scholar - AV Kildishev, A Boltasseva, VM Shalaev, Planar Photonics with Metasurfaces. Science
**339**(6125), 1232009 (2013)View ArticleGoogle Scholar

## Copyright

This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.